Incommensurate modulation and thermal expansion of Sr~3~B~2+x~Si~1-x~O~8-x/2 solid solutions
Volkov, Sergey; Bubnova, Rimma; Bolotina, Nadezhda; Krzhizhanovskaya, Maria; Belousova, Olga; Filatov, Stanislav; Acta Crystallographica, Section B: Structural Science, Crystal Engineering and Materials 71 (2015) 489–497; doi:10.1107/S2052520615011713

data_2310767
_publ_section_title
;
 Incommensurate modulation and thermal expansion of
 Sr~3~B~2+x~Si~1-x~O~8-x/2 solid solutions
;
_journal_coden_ASTM              ACSBDA
_journal_coeditor_code           DK5034
_journal_issue                   5
_journal_name_full
;
 Acta Crystallographica, Section B: Structural Science, Crystal Engineering
 and Materials
;
_journal_page_first              489
_journal_page_last               497
_journal_paper_doi               10.1107/S2052520615011713
_journal_volume                  71
_journal_year                    2015
_chemical_formula_sum            'B3.041 O10.479 Si0.959 Sr4'
_chemical_formula_weight         577.9
_chemical_name_systematic        ' ?'
_space_group_IT_number           62
_symmetry_cell_setting           orthorhombic
_symmetry_space_group_name_Hall  '-P 2ac 2n'
_symmetry_space_group_name_H-M   'P n m a'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            1
_cell_length_a                   12.2774
_cell_length_b                   3.9006
_cell_length_c                   5.4091
_cell_measurement_temperature    293
_cell_volume                     259.038
_diffrn_ambient_temperature      293
_diffrn_measured_fraction_theta_full 0.98
_diffrn_measured_fraction_theta_max 0.96
_diffrn_radiation_source         'X-ray tube'
_diffrn_radiation_type           'Mo K\a'
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.1069
_diffrn_reflns_limit_h_max       23
_diffrn_reflns_limit_h_min       -23
_diffrn_reflns_limit_k_max       7
_diffrn_reflns_limit_k_min       -7
_diffrn_reflns_limit_l_max       3
_diffrn_reflns_limit_l_min       -9
_diffrn_reflns_number            8190
_diffrn_reflns_theta_full        36.74
_diffrn_reflns_theta_max         43.24
_diffrn_reflns_theta_min         4.12
_exptl_absorpt_coefficient_mu    20.637
_exptl_crystal_density_diffrn    3.7048
_exptl_crystal_F_000             264
_refine_diff_density_max         3.58
_refine_diff_density_min         -5.05
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   2.34
_refine_ls_number_constraints    1
_refine_ls_number_parameters     29
_refine_ls_number_reflns         1031
_refine_ls_number_restraints     0
_refine_ls_R_factor_all          0.2015
_refine_ls_R_factor_gt           0.0765
_refine_ls_shift/su_max          0.0012
_refine_ls_shift/su_mean         0.0003
_refine_ls_structure_factor_coef F
_refine_ls_weighting_details     w=1/(\s^2^(F)+0.0001F^2^)
_refine_ls_weighting_scheme      sigma
_refine_ls_wR_factor_gt          0.0772
_refine_ls_wR_factor_ref         0.0907
_reflns_number_gt                428
_reflns_number_total             1031
_reflns_threshold_expression     I>3\s(I)
_cod_data_source_file            dk5034sup1.cif
_cod_data_source_block           I
_cod_original_cell_volume        259.0376
_cod_original_sg_symbol_Hall     '-P -2xabc;-2yb;-2zac'
_cod_database_code               2310767